### compounds

### Thesis submitted for the degree of

### Doctor Philosophiae

### CANDIDATE:

### SUPERVISOR:

### Matteo Cococcioni

### Stefano de Gironcoli

Introduction 4

1 Theoretical tools and approximations 7

1.1 The Born Oppenheimer approximation . . . 7

1.2 Density Functional Theory . . . 9

1.2.1 Approximations for the exchange-correlation energy functionals: LDA and GGA . . . 13

1.2.2 The Local Spin Density Approximation . . . 14

1.3 Periodic systems: the Bloch theorem . . . 16

1.4 The plane wave pseudopotential method . . . 18

1.4.1 The non linear core correction . . . 22

2 Some d-open shell systems studied with GGA 24 2.1 introduction . . . 24

2.2 Bulk iron . . . 26

2.3 Iron oxide . . . 30

2.4 Fe2SiO4 Fayalite . . . 39

3 The LDA+U method within a PW PP framework 50 3.1 Introduction . . . 50

3.2 Rotational invariant LDA+U method . . . 53

3.3 LDA+U simplified scheme . . . 56

3.4 Calculating the Hubbard U . . . 60

3.5 Implementation of the LDA+U approach in a PW PP code . . . 68

4 The LDA+U approach: application to some real systems 70 4.1 Bulk iron . . . 71

4.2 Iron oxide . . . 85

4.3 Fe2SiO4 fayalite . . . 98

5 Conclusions 108

Since its theoretical foundation in the mid-1960’s [1, 2], Density Functional Theory (DFT) has demonstrated a large predictive power in the study of the ground states properties of real materials, so that it has soon become the most important tool (if not the only one) for first principles calculations. Though exact in principle, this theoretical scheme needs some approximations to be used in practical calculations. In fact, the many body problem concerning an interacting electron system is far too complicated to be approached directly, so that it is usually treated in a simpler one body formalism which describes a fictitious non interacting electron gas with the same density of the real interacting one. In this simplified scheme the many body contributions to the electronic interactions are usually modeled in some approximations.

The simplest of these simplified (and the first historically introduced) is the Local (Spin) Density Approximation (LSDA) which is based on the assumption that the elec-tronic system can be locally represented by a uniform electron gas with the same density. Using L(S)DA the structural, electronic and magnetic ground state properties of a large class of materials, including, for instance, nearly-free-electron-like (simple) metals, cova-lent semiconductors, ionic solids, and even rather complex intermetallic transition metal compounds, could be described and understood very deeply and usually within a fair agreement with experimental results.

A possible extension to the LDA method is represented by (spin-polarized) General-ized Gradient Approximation (GGA approaches) which, in the modeling of the effective electronic interactions, also accounts for the possible inhomogeneity of real electron sys-tems. The introduction of this approach could solve indeed some open questions within LSDA and even improve the descriptive power of DFT calculations about the structural and the electronic properties of some real non homogeneous systems as, for instance, the transition metal compounds.

However GGA functionals brought out very little enlargement of the class of materi-als whose properties could be successfully described by DFT, so that there still remains

of materials mainly consists in the fact that their energy functionals are built treating the real interacting electron system as a (possibly homogeneous) electron gas, and thus result to be not accurate enough to deal with situations in which strong localization of the electrons is likely to occur. The description and understanding of the electronic structure of strongly correlated materials is indeed a very long standing problem and the transition metal oxides (which, in contrast with the observed insulating behavior, are incorrectly predicted to be metals or small gap semiconductors by LSDA or GGA) have represented for long time the most notable failure of DFT. When the high-Tc

supercon-ductors entered the scene (their parent materials are also strongly correlated systems) the study of new approaches which could allow to describe this kind of systems with first principle calculations received a new impulse, and in the last fifteen years many methods were proposed in this direction.

One of the most popular approaches of this kind is LDA+U for which a variety of different functionals were introduced and developed. Although the different formulations can differ, to some extent, from each other for their theoretical construction and the technical details concerning their practical implementation, the main idea they all rely on is the same and mainly consists in trying to correct the standard (LDA or GGA) energy functionals with a mean field Hubbard-like term which is meant to improve the description of the electronic correlations. The formal expression of this additional energy functional is generally taken from the model hamiltonians (the Hubbard model is just one example) that represent the ”natural” theoretical framework to deal with strongly correlated materials. These models, however, are strongly dependent on the choice of the interaction parameters which sometimes have been evaluated using ab-initio (constrained) calculations. Anyway, no general procedure is well established to calculate these effective interaction parameters entering the theory and this situation is also reflected in the LDA+U-like approaches. In fact, the few method which have been proposed to extract the effective electronic interactions from first principle (constrained) calculations, did not give very reliable results, so that their value is usually determined by seeking a good agreement of the calculated properties with the experimental results in a semiempirical way.

In this work a critical study of the LDA+U approach is proposed, which starting from the formulation of Anisimov al. [3, 4, 5], and its further improvements [6, 7, 8], develops

a simpler approximation that appears, to our opinion, a more ”natural” extension of the LDA (or GGA) description we aim to correct and complete. In this context a method to calculate the interaction parameters is also introduced which is based on a linear response approach and allows to fix the parameters entering the LDA+U correction in close relationship with the behaviour of the system under consideration, without any aprioristic assumption.

This methodology is then applied to the study of the electronic, magnetic and struc-tural properties of some iron compounds, chosen as representative of ”normal” (bulk iron) and strongly correlated (iron oxide and fayalite) situations.

The present thesis is organized as follows. After having devoted a first chapter to a brief overview of the standard DFT techniques and approximations, in the second chapter we present results about the electronic, magnetic, and structural properties of some iron compounds obtained within the GGA framework. We underline the merits of this approach in describing these crystals, but also point out the aspects which need a further improvement to be correctly described because the relevance of strong electronic correlation. In the second chapter the LDA+U method and its implementation within a pseudopotential-plane wave framework are introduced. We start from a brief historical overview about this theoretical method and discuss the goals it was built for. Then we focus on the particular approximation we actually use and underline the motivations which led us to consider this simpler expression for the LDA+U functional. To complete the theory and make our approach self-sustaining, a linear response approach to calculate the effective electronic interactions entering the LDA+U correction is also presented, together with a discussion about the differences with the approaches presented in other works. In the fourth chapter we deal with the same systems studied in the second chapter but using LDA+U. We focus on the improvements we obtain with respect to the GGA calculations and discuss the role of LDA+U corrections in describing the electronic structure of these materials and their structural properties. A conclusive discussion about merits and defects of the presented simplified LDA+U scheme and of the linear response approach to calculate the effective interactions is presented in the last chapter together with some possible perspectives of improvement and still remaining problems.

### Theoretical tools and

### approximations

In this chapter the theoretical approaches and approximations used in standard first principles calculations will be briefly described. Our motivation is twofold: on one hand the most commonly used tools employed in the study of the physical properties of real materials are reminded; on the other hand a more complete description is given to the theoretical background our LDA+U approach is built on. This will provide a better understanding of the starting point of the new theoretical approach and a good knowledge of the many technical details required for its practical implementation.

### 1.1

### The Born Oppenheimer approximation

The possibility of treating separately the electrons and the ions of a real system, ab-initio calculations generally rely on, is the result of the adiabatic approximation of Born and Oppenheimer [11] which is a consequence of the large mass difference between the two families of particles. In other words, being much lighter than the ions, the electrons can move in a solid much faster than the nuclei and the electronic configuration can be considered as completely relaxed in its ground state at each position the ions assume during their motion. In mathematical terms we would say that the time scale for the electron excitations, the inverse of their bandwidth, is usually much smaller than the one for the ions, namely the inverse of the phonon frequencies. This means that while studying the electronic degrees of freedom the ions can be considered at rest; thus the total wavefunction of the system can (approximately) be written as the product of a function describing the ions and another for the electrons depending only parametrically

upon the ionic positions:

Ψ(R, r) = Φ(R)ψR(r) (1.1)

where R = {RI} is the set of all the nuclear coordinates, and r = {ri} is the same

quan-tity for all the electrons in the system (though not explicitly indicated, the many particle wavefunction ψR(r) also depends on the electronic spin degrees of freedom). Within this

approximation, the ionic wavefunction Φ(R) is the solution of the Schr¨odinger equation: −X I ¯ h2 2MI ∂2 ∂R2 I + E(R) ! Φ(R) = εΦ(R) (1.2)

where MI is the mass of the Ith nucleus and E(R) is the so called Born-Oppenheimer

potential energy surface corresponding to the ground state energy of the electronic system when the nuclei are fixed in the configuration R. More generally electronically excited potential energy surfaces can be defined which are important when electronic transitions driven by ionic motion, through the non adiabatic coupling terms (electron-phonon interaction), are considered. The potential energy surface can be computed solving the Schr¨odinger problem for the electrons:

−
X
i
¯
h2
2m
∂2
∂r2
i
+e
2
2
X
i6=j
1
|ri− rj| −
X
iI
ZIe2
|ri− RI|
+ e
2
2
X
I6=J
ZIZJ
RI− RJ
ψ_{R}α(r) =
= Eα(R)ψαR(r) (1.3)

where ZI is the charge of the Ith nucleus, −e and m are the electronic charge and mass,

and α is an index for the electronic state.

The equations describing the electronic and the ionic problems are obtained from the equation for the total system assuming the wavefunction factorization of eq. 1.1 and neglecting the non adiabatic terms which come from the kinetic operator for the nuclei acting on the electronic wavefunction ψR(r). This is expected to be a good

approximation for most real materials since the neglected terms are of the order of the ratio me/M between the (effective) electronic mass and the ionic one. The separation

among electronic and ionic degrees of freedom is a very useful simplification of the problem and allows to treat the ions within a classical formalism as generally done in molecular dynamics calculations. However the electronic problem is a quantum many body problem; the total wavefunction of the system depends on the coordinates of all the electrons and cannot be decoupled in single particle contributions because of their mutual interaction, so that the problem is still far too complicated to be solved exactly in practical computations. Owing to this difficulty, further developments are required to perform ab-initio calculations for real materials. Density Functional Theory provides a framework for these developments.

The first important conceptual advantage introduced by Density Functional Theory (DFT) [1] is the possibility to describe the ground state properties of a real system in terms of its ground state electronic charge density (which depends on just one spatial variable) instead of the far more complicated wavefunctions (which depends on the coordinates of all the electrons in the system). Dealing with the charge density allows to reformulate the problem in a mean-field-like language which is however based on an exact result. If we consider an interacting electron gas, the external potential acting on the particles determines the ground state of the system and the corresponding charge density. Thus, all the physical quantities concerning this state (like, for instance, the total energy) are functionals of the external potential. As it was first demonstrated by Hohenberg and Kohn [1], due to a one to one correspondence among the external potential and the ground state density (which allows to express the former as a functional of the latter), there also exists a unique universal functional F [n(r)] of the ground state electron density alone such that a variational principle exists with respect to the electron density for the total energy functional

E[n(r)] = F [n(r)] + Z

Vext(r)n(r)dr (1.4)

where F [n(r)] contains the kinetic energy and the mutual Coulomb interaction of the electrons, and Vext(r) represents the external potential acting on the particles. The

minimization of this functional with the condition that the total number of particles, N , is preserved:

Z

n(r)dr = N, (1.5)

directly gives the ground state energy and charge density, from which all the other physical properties can be extracted. This variational principle is very important from a conceptual point of view as it suggests a procedure to access all the interesting quantities. Unfortunately, the universal functional F [n(r)] (which is independent on Vext(r))

is not known in practice and in order to transform DFT into a useful tool Kohn and Sham [2] introduced a further development which consists in mapping the original in-teracting problem into an auxiliary non inin-teracting one. For this fictitious system of non interacting electrons the Hohenberg and Kohn theorem also applies and the unique functional F [n(r)] corresponds in this case to the kinetic energy of the non interacting electrons, T0[n(r)]. The density functional F [n(r)] for the interacting system can then

the same density of the real one and the additional terms describing the interparticle
interaction:
F [n(r)] = T0[n(r)] +
e2
2
Z n(r)n(r0)
|r − r0_{|} drdr
0_{+ E}
xc[n(r)]. (1.6)

The second term in the right hand side of eq. 1.6 is the classical Coulomb interaction among the electrons described through their charge density (the Hartree term), whereas Exc[n(r)] is the so called exchange-correlation energy and accounts for all the many body

effects which are not described in the other terms. In practice this term contains all the differences among the non interacting fictitious system and the real interacting one (here including corrections for the Coulomb interaction and for the kinetic energy also) so that what we do is confining our ignorance about F [n(r)] into one single, hopefully small, term. This is particularly useful when we minimize the functional F [n(r)] with the constraint given by the conservation of the total number of particle to obtain the ground state physical properties of the real system. In fact from eq. 1.6 it is quite easy to extract the effective potential VKS acting on the electrons of the fictitious non

interacting system. If we impose the total energy functional for the non interacting electron gas E0[n(r)] = T0[n(r)] + Z VKS(r)n(r)dr − µ0 Z n(r)dr − N (1.7) to be minimized by the same electron density which also minimizes the total energy of the interacting electron system

E[n(r)] = T0[n(r)] +
e2
2
Z n(r)n(r0)
|r − r0_{|} drdr0+ Exc[n(r)] +
Z
Vext(r)n(r)dr − µ
Z
n(r)dr − N
(1.8)
the expression for the effective Kohn-Sham potential results:

VKS(r) = Vext(r) + e2
Z n(r0)
|r − r0_{|}dr
0_{+ v}
xc(r), (1.9)
vxc(r) =
δExc[n]
δn(r) , (1.10)

which is defined within an unimportant additive constant corresponding to the difference
among the chemical potentials µ and µ0_{, which were introduced in the total energy}

functionals as Lagrange multipliers to ensure the conservation of the total number of particles. The resulting effective hamiltonian for the system is the one describing a non interacting electron gas feeling the effective potential VKS in which all the interparticle

to be written as:

n(r) =X

i

fi|ψi(r)|2, (1.11)

where i is an index for the single particle state, and fi is the Fermi distribution (which

corresponds to θ(F−i) for T = 0). The kinetic energy for the non interacting auxiliary

system is also straightforward to compute within this formalism:
T0[n(r)] = −
X
i
fi
Z
ψi∗(r)
¯
h2_{∇}2
2m ψi(r)dr. (1.12)

From the minimization of the non interacting energy functional with respect to ψ∗ i

with the constraint of fixed number of electrons, the following set of Schr¨odinger-like equations (called Kohn-Sham equations) can be obtained:

ˆ HKSψi(r) = " −¯h 2 ∇2 2m + VKS(r) # ψi(r) = iψi(r) (1.13)

where the hermeticity of the operators appearing in this expression ensures the possi-bility of choosing the constraints in such a way the orthonormality conditions for the fictitious wavefunctions are satisfied:

Z

ψ∗i(r)ψj(r)dr = δij. (1.14)

It is worth to remark that the wavefunctions appearing in the Kohn-Sham equations have no direct physical meaning: they are the eigenstates of the one body density matrix we use in the theory but cannot be considered the wave functions for the electrons of the real system as they are the electronic orbitals for the auxiliary non interacting gas. The set of the Kohn-Sham equations is a strongly non linear one since the electronic wavefunctions, which are to be obtained as the solutions of the problem, also enter the expression of the effective potential as they are used in building the charge density on which VKS depends.

This means that, in order to solve this system, we have to adopt an iterative method which, starting from an initial guess for the wavefunctions and the potential, evolves both quantities up to self consistency. Owing to the fact that solving the Kohn-Sham equations corresponds to minimize the total energy functional of the N -electrons system on a set of orthonormal single particle wavefunction, the ground state total energy can also be expressed as:

E0[n(r)] =
X
i
fii−
e2
2
Z n(r)n(r0)
|r − r0_{|} drdr0+ Exc[n(r)] −
Z
vxc(r)n(r)dr + Eion (1.15)

where the Hartree (H) and the exchange-correlation (xc) contributions respectively ac-count for the double ac-counting and the misac-counting of the same quantities in the sum of the eigenvalues, whereas Eion is the energy term accounting for the direct Coulomb

interaction among the ionic cores. The variational principle the theory relies on, eq. 1.8,
implies that the total energy functional is quadratic, near the self consistent point, in
the fluctuations of the wavefunctions (or the charge density) around their self consistent
value. This variational properties is not shared by eq. 1.15 which displays a linear error
near the self consistent point. In fact, at any intermediate step of the minimization, the
Hxc potential entering the expression of the Kohn-Sham hamiltonian, eqs. 1.13 and
1.9, is calculated from the charge density nin _{obtained in the previous iteration. This}

charge density is generally different from the analogous quantity obtained in the current
diagonalization nout_{. The sum of the eigenvalues thus reads:}

Eband = X i fii = T0[nout] + Z (Vext(r) + VHxcin (r))n out (r)d(r) (1.16) which behaves at most linearly in the above mentioned fluctuations of the quantity nout

around its self consistent value. To obtain a variational total energy we can add some
corrections to the band energy which eliminate the undesired dependence on nin_{. The}

final expression results:
˜
Eband[nout] =
X
i
fii +
Z
(VHxcout(r) − V
in
Hxc(r))n
out
(r)d(r) =
T0[nout] +
Z
(Vext(r) + VHxcin (r))n
out_{(r)d(r) +}Z _{(V}out
Hxc(r) − V
in
Hxc(r))n
out_{(r)d(r) =}
T0[nout] +
Z
(Vext(r) + VHxcout(r))n
out
(r)d(r) (1.17)

where it is evident that the correction (to be added to E0 in eq. 1.15) completely vanish

when self consistency is reached (full details can be found in [12]).

The theoretical approach described so far is expected to be very efficient when the dominant part of the energy consists of the kinetic and the electrostatic terms be-cause they are described without any approximation. However the success in studying real materials depends very strongly on how the (hopefully small) exchange-correlation contribution is described and this is particularly true with systems (like the strongly correlated materials studied in this thesis) where the many body effects are expected to be important.

### tionals: LDA and GGA

Up to this point no approximation was introduced into the theory, but there still ex-ists a term (the exchange-correlation energy) which, though well defined (and exact) in principle, has a very complicated expression which is not known explicitly. Some assumptions are thus needed in the definition of Exc to convert the DFT in a practical

tool for ab-initio calculations and this modeling necessarily introduce in the theory some approximations.

The simplest of these descriptions is called the Local Density Approximation (LDA) and is obtained assuming that the xc energy of a real system behaves locally as in a uniform (homogeneous) electron gas having the same density. The xc energy thus depends only on the local density of the system and actually reads:

ELDA xc [n] = Z εhom xc (n(r))n(r)dr (1.18) where εhom

xc (n(r)) is the xc energy density of the above mentioned homogeneous system.

The xc potential can be easily obtained from the xc energy functional and results: vxcLDA(r) = δELDA xc [n] δn(r) = ∂Fxc(n) ∂n |n=n(r) (1.19) where Fxc(n) = εhomxc (n)n. This approximation was designed to work with systems in

which the electronic charge density is expected to be smooth (like, for instance, in nearly free-electron-like (simple) metals, intrinsic semiconductors and so on) but it gives indeed quite good results also with non homogeneous systems like covalently bonded materials and (some) transition metals. It typically produces good agreement with experiments about structural and vibrational properties, but usually overestimates bonding energies and predicts shorter equilibrium bond lengths than found in experiments. In order to overcome these and other difficulties of LDA, some extensions of the original approxi-mation were introduced among which the Generalized Gradient Approxiapproxi-mation (GGA) family is one of the most successful. Within GGA the xc energy is a functional not of the density alone, but also of its local spatial variations:

ExcGGA[n] =

Z

εGGAxc (n(r), |∇n(r)|)n(r)dr. (1.20)

Several expressions of the xc energy density have been described in different formulations of the GGA functionals. Among these, the Perdew-Burke-Ernzherof (PBE) expression was chosen in this work [13].

The potential corresponding to the energy functional EGGA

xc [n] can be expressed as:

vxcGGA(r) = δEGGA xc [n] δn(r) = ∂Fxc ∂n − 3 X α=1 ∂α ∂Fxc ∂(∂αn) !! |n=n(r) (1.21)

where Fxc(n, |∇n|) = εGGAxc (n, |∇n|)n, ∂α stands for the αth component of the gradient

and the rule of integration by parts was used to obtain the last equality. This improved approximation is actually able to cure some defects of LDA and generally produces better description of the structural properties of real materials. In particular it improves significantly the results about the binding energy of real system. It is also expected to give a better description of non homogeneous systems, like transition metals, producing correct results in some cases where LDA completely fails. One example is bulk iron which in agreement with experiments, is predicted by GGA to have a ferromagnetic (FM) bcc ground state rather than a paramagnetic fcc one as found in LDA.

Despite the theory is exact in principle, the approximations we have to adopt for the exchange and correlation energy both in LDA and GGA introduce a mean-field-like formalism which can be expected to work well for systems with rather delocalized electrons but is not sufficiently accurate when dealing with materials with localized electrons for which many body effects are expected to be more important.

### 1.2.2

### The Local Spin Density Approximation

A formulation of the xc functional depending only on the total electron density should allow an exact description of real materials; however the treatment of magnetic systems is much simpler if the xc energy functional is explicitly considered as dependent on the two spin populations separately. In this case the Kohn Sham equations can be written independently for the two spin polarizations:

"
−¯h
2
∇2
2m + V
σ
KS(r)
#
ψσ
i(r) = σiψiσ(r) (1.22)
where we have:
Vσ
KS(r) = Vext(r) + e2
Z n(r0)
|r − r0_{|}dr
0_{+ v}σ
xc(r) (1.23)
vxcσ (r) =
δExc[n↑, n↓]
δnσ_{(r)} (1.24)
nσ_{(r) =} X
i
fσ
i |ψ
σ
i(r)|
2_{,} _{n(r) =}X
σ
nσ_{(r).} _{(1.25)}

Of course the two spin populations interact with each other through the Hartree and xc potentials and the effective field acting on one of them depends on the opposite-spin charge density also. As it can be observed from the expression of the effective

the unbalance between up and down spin states, which originates the magnetization, is indeed produced by the exchange and correlation potential which accounts for the differences between like-spin and unlike-spin interactions. The exchange and correlation functionals of this generalized spin-dependent approach (whose simplest variant is the so called Local Spin Density Approximation) are usually given separate expressions. In fact, the exchange contribution is diagonal in the spin and can be obtained extending the non polarized expression:

ExLSDA[n] = X σ Z FxLSDA(nσ(r))d~r = X σ 1 2 Z FxLDA(2nσ(r))d~r (1.26) where FLDA

x is the same functional used for the unpolarized case. The correlation

functional, instead, is obtained interpolating the results for the homogeneous electron gas at different spin polarizations and can be written as dependent on both the (total) charge density n(r) and the magnetization m(r) which is defined as:

m(r) = µB(n↑(r) − n↓(r)). (1.27)

If we define the magnetic polarization, ξ(r) =

1

µB|m(r)|

n(r) , (1.28)

so that 0 ≤ ξ ≤ 1, this contribution to the total energy actually results:
ELSDA
c [n, ξ] =
Z _{h}
U
c(n(r)) + f (ξ(r))
P
c(n(r)) − Uc(n(r))
i
n(r)dr (1.29)
where f (ξ) is a smooth interpolating function with f (0) = 0 and f (1) = 1, and the
P

c and Uc functionals represent respectively the correlation energy densities for the

polarized and the unpolarized systems. The contribution to the Kohn-Sham potential coming from the exchange and correlation functionals described so far corresponds to an effective magnetic field. In fact, by calculating the first derivative of these quantities with respect to the spin polarized charge densities, we obtain a first term equal for the two spin polarizations and a second one (depending on the magnetization) which has the same absolute value but changes sign according to the spin it is applied on. This latter term introduces differences in the two effective fields thus producing the spin unbalances from which the magnetic properties of the system derive.

A similar extension to the spin polarized case is also possible within the GGA ap-proximation. However, within this approach, the correlation contribution usually does

not contain the gradient of the magnetic polarization [13] and the functionals finally
reads:
Eσ−GGA
x =
1
2
X
σ
Z
Fx(2nσ, |2∇nσ|)dr (1.30)
Eσ_{−GGA}
c =
Z
Fc(n, ξ, |∇n|)dr (1.31)

where Fx and Fc are the gradient-dependent analogues of the quantity defined in the

LDA case.

### 1.3

### Periodic systems: the Bloch theorem

The description of real (bulk) materials within ab-initio calculations is based on the assumption that the atoms which compose them are at rest in their equilibrium positions and these form an infinite, periodically repeated structure. In mathematical terms, if we call V the external potential acting on the electrons, we have:

V (r + R) = V (r) (1.32)

where R is a direct lattice vector corresponding to an integer linear combination of three fundamental vectors determining the periodicity of the lattice in three independent directions. The whole electronic hamiltonian and all the physical quantities describing the periodical system also share the translational invariance of the lattice and this allows to use the Bloch theorem which states that the single particle electronic wave function can be expressed in the form

ψkv(r) = eik·rukv(r) (1.33)

where k is the crystal momentum of the electrons (it actually describes the translational properties of the wavefunction), v is a discrete index (called the band index) classifying states corresponding to the same k−vector and ukv(r) is a function with the same

periodicity of the crystal:

ukv(r + R) = ukv(r). (1.34)

Due to the translational invariance of the system different k−points can be treated independently. In fact, the hamiltonian commutes with the operators which generate translations through the points of the lattice and is thus block diagonal on the basis set of the eigenvectors of these latter operators which corresponds to Bloch wavefunction of the form given in 1.33 and are classified by k. In this context the band index v numbers the eigenvalues of the hamiltonian belonging to the same k−block.

reciprocal space which has a periodic structure whose fundamental lattice vectors bi are

related to the ones of the real (direct) space ui as follows:

bi· uj = 2πδij i, j = 1, 2, 3. (1.35)

The sums over the electronic states which define many physical quantities as, for in-stance, Eband and n(r), actually correspond to integrals over the BZ (and sums over the

band index v). Using the symmetry of the crystal, the integration can be conveniently
confined in a smaller region of the BZ, the so called irreducible wedge of the Brillouin
zone (IBZ). This result can be further improved by the use of the special point
integra-tion technique which allows to perform reciprocal space integraintegra-tion (needed for example
when calculating the charge density or the sum of the eigenvalues) using generally a
small set of k-vectors in the IBZ. These points can be chosen according to different
techniques [14](in this thesis we use the Monkhorst and Pack recipe) and in general the
accuracy of the (approximate) method can be checked by the convergence properties of
the physical properties of interest upon increasing their number. As an example, the
reciprocal space integration for the charge density is performed as a sum over a discrete
set of vectors:
˜
n(r) = X
k_{∈IBZ}
ωk
X
v
fkv|ψkv(r)|2 (1.36)

from which the electronic charge density results through a symmetrization procedure:
n(r) = 1
NS
X
S
˜
n(S−1r_{− f)} (1.37)

where NS is the number of symmetry operations S in the space group of the crystal and

f a possible fractional translation. In eq. 1.36 the ωk coefficient is the k-point weight

calculated within the special point technique.

The special points technique is very efficient in the description of semiconductors or insulators but gives poor results when directly applied to metals. This happens because the region around the Fermi level (which is crossed by some electronic states) needs to be sampled quite accurately and in general a larger number of vectors is required. If the used k-point grid is not fine enough, there could also be problems of instability during the self-consistent run because even small shifts in the Fermi energy could include or exclude in the reciprocal space sums (like the one in eq. 1.36) a finite number of electronic states thus producing considerable fluctuations in the corresponding quantities. A possible so-lution to this problem can be achieved using the tetrahedron method which consists in

decomposing the BZ into symmetry breaking elemental volumes and connecting the en-ergy bands between neighboring k-points by linear interpolation. However this method presents some important drawbacks [15] so that we choose to use another approach to the problem of describing metallic systems. This technique consists in introducing a finite smearing of the Fermi distribution (actually corresponding to consider a finite effective temperature) which smoothes the weight of the states around this level and avoids large fluctuations in the calculated quantities. The convoluting function used to introduce the smearing can be chosen in many ways: finite temperature Fermi distri-bution, Lorentzian, Gaussian [16], cold smearing factors [17], and so on. In this thesis the Methfessel and Paxton smearing technique [18] is used which adopts a combination of Gaussians and polynomials as spreading functions. This approximation works quite well for metals (even if a larger number of k-points is usually required than for semi-conductors) and the accuracy of the reciprocal space integrations at finite smearing can be checked by their convergence properties upon increasing the number of the special k-vectors in the IBZ and reducing the broadening width σ. The main drawback intro-duced by the smearing technique is the dependence of the ground state total energy on the chosen σ. The Methfessel and Paxton methods allows to considerably reduce this dependence by accurately choosing the convoluting function to smear the Fermi distribution.

### 1.4

### The plane wave pseudopotential method

In order to solve the KS equations by practical calculations we need to transform the original integro-differential problem into a more tractable algebraic one. This can be achieved by expanding the electronic wavefunctions on a basis set and using this rep-resentation in all operators in the hamiltonian. The one chosen in this work (and one of the most used in ab-initio calculations) is the Plane Wave (PW) basis set [12] which takes advantage from efficient algorithms, like the Fast Fourier Transform (FFT), to move back and forth from real to reciprocal space. The Bloch electronic wave function in eq. 1.33 can thus be represented in the form:

ψkv(r) =
1
(N Ω)12
X
G
ei(k+G)·r_{c}
v(k + G) (1.38)

where Ω is the volume of the unit cell, the G vectors are the reciprocal lattice vectors, and the cv(k + G) coefficients are normalized in such a way that:

X

G

X
G0
"
¯
h2
2m|k + G|
2 _{+ v}
h(G − G0) + vxc(G − G0) + vext(G, G0)
#
cv(k + G0) = kvcv(k + G).
(1.40)
It is evident from this expression that the hamiltonian has block diagonal form with
respect to the k vectors and the diagonalization can thus be performed within each of
these block separately. As we are studying the ground state properties of the system,
for each k−point only a finite number of the lowest-energy electronic states on which
all the electrons of the system can be accommodated, need to be computed to obtain
the charge density. This quantity is then used to construct a new guess of the potential
to be reintroduced in the Kohn-Sham equations for the successive step of the iterative
diagonalization. Of course the PW expansion is exact in the limit of infinite number
of G-vectors. In practical calculations one can deal only with a finite number of plane
waves and usually chooses those contained in a sphere of maximum kinetic energy Ecut

(the energy cut-off):

¯ h2

2m|k + G|

2

≤ Ecut. (1.41)

The accuracy we obtain in resolving the KS equation under the condition in eq. 1.41 has to be checked each time by increasing the value of the energy cut-off and studying the convergence of the properties we are interested in. The big advantage of using the PW expansion mainly consists in the fact that Ecut is the only parameter in the theory

which controls the accuracy of the description of the system under consideration. This means that, once Ecut is fixed, all the wavefunctions of the system whose variation takes

place over distances larger than (and up to) 2π¯h/√2mEcut can be well described.

Unfortunately, the PW expansion uses the same resolution in each region of space so that, to describe the ionic cores and the electronic states partially localized around them, we would need an intractably large number of G vectors. One possible way around this difficulty is the Pseudopotential (PP) technique, which is based on the assumption that the most relevant physical properties of a system, as far as bonding and chemical reactiv-ity are concerned, are brought about by its valence electrons only, while the ionic cores (the nuclei dressed by the most internal electronic cloud) can be considered as frozen in their atomic configurations. The valence electrons thus move in the effective external field produced by these inert ionic cores and the pseudopotential tries to reproduce the interaction of the true atomic potential on the most external (valence) states without explicitly including the core states in the calculations. There exist different procedures to build a pseudopotential but the general ideas they rely on are similar. Once a full

potential calculation is performed for the isolated atom, the electronic states are divided into two categories: the internal states and the valence ones. The internal electrons re-main frozen in their ground state atomic configuration whereas for the external ones a pseudowavefunction is built (which matches the corresponding full potential one in the region external to a fixed core radius) which is chosen to be smooth and nodeless inside the core, while conserving the total valence charge in this region (norm conserving condi-tion). Given a choice for both the core radius and the shape of the pseudowavefunction, a pseudopotential is built (inverting the Schr¨ondinger-like equation for the considered electronic state) which reproduces the scattering properties of the ”real” valence states of the reference atomic configuration in a region of energies which has to be as large as possible in order to give good transferability of the pseudopotential when used in different chemical environments. Owing to the smoothness of the pseudowavefunction, the calculations can be performed with a reasonable number of plane waves. However in order to reproduce the scattering properties of the all-electrons (AE) wavefunctions of several angular momenta, it is usually necessary to split the pseudopotential in a local part (matching the real full potential outside the core) and a non local one (vanish-ing outside the core) which acts in different ways on each different angular momentum channel. The first expression for this non local contribution was given in a semi-local form [19, 20, 21] where the non-locality is built just on the angular coordinates:

V (r, r0) = Vloc(r)δ(r − r0) + lmax

X

l=0

Vl(r)δ(r − r0)Pl(r, r0), (1.42)

where Pl is the projector operator onto the lth angular momentum subspace. However,

in order to make the PW calculation more efficient, Kleinman and Bylander (KB) [22] replaced the above semilocal expression with a fully separable form:

V (r, r0) = Vloc(r)δ(r − r0) +

X

i

|iiVihi|. (1.43)

where the wavefunctions |ii are (modified) atomic pseudo-states such that the KB po-tential reproduces the action of the original semilocal one on the reference atomic pseu-dowavefunctions.

The most complete generalization (and improvement) of this scheme was introduced by Vanderbilt [23, 24] who found a method to increase the transferability of the PPs while reducing the workload necessary to describe the pseudowavefunctions inside the cores. The region of energy corresponding to occupied states in the crystals is sampled with more than one projector so that the index i in eq. 1.43 runs not just on the atomic

values around them used to reproduce the correct scattering properties of the ion. This requires a generalization of the expression 1.43 whose non local part becomes:

Vnl =

X

i,j

Bij|βiihβj| (1.44)

where the functions |βii are built from the chosen pseudowavefunctions (corresponding

to the chosen energy i) and local pseudopotential and are localized in the core region

(they vanish at a chosen core radius of the atom on that site), while the matrix Bij

is an hermitian operator built using the same quantities. This is already a very useful improvement as it allows to increase the PP transferability, but the most important reduction of the computational load introduced by the ultrasoft (US) PPs comes from the relaxation of the norm conserving condition on the pseudowavefunctions and the possibility of choosing them as smooth as possible inside the core regions. This is possible by introducing a generalized overlap operator:

S = 1 +X

i,j

qi,j|βiihβj| (1.45)

so that the orthonormality condition to be satisfied in the solution of the KS equations is:

hψi|S|ψji = δij. (1.46)

In these expressions qi,j is the integral of the augmentation charge density,

qi,j =
Z
Qi,j(r)dr (1.47)
Qi,j(r) = ψiAE∗(r)ψ
AE
j (r) − ψ
P S_{∗}
i (r)ψ
P S
j (r) (1.48)

where the wavefunctions appearing in eq.1.48 are the atomic (all-electrons and pseudo) states used to build the crystal electronic ones. Owing to this generalization of the overlap, the charge density has to be completed with the augmentation part on the ionic cores: n(r) =X k,v fkv |ψkv(r)|2+ X I,i,j QIij(r − RI)hψkv|βiIihβ I j|ψkvi . (1.49) In this expression an index, I, counting the different ions, in position RI has been added

to the augmentation charges QI

ij and to the β functions. This modification in n(r) also

involves the expression of the potential in the KS equations. If we describe the external potential in the form:

V (r, r0) = Vloc(r)δ(r − r0) + X I,i,j DijIion|β I iihβ I j| (1.50)

the coefficient DIion

ij have to be calculated as:

DIionij = B I

ij+ jqijI (1.51)

and the KS equations (which have to be solved with the generalized orthonormality condition 1.46) finally read:

−∇ 2 2 + X I,i,j DIij|β I iihβ I j| + Vef f |ψkvi = kvS|ψkvi (1.52) where Vef f = Vloc+ VHxc and DIij = D Iion ij + Z Vef f(r)QIij(r − R)dr. (1.53)

As evident from the last expression, the pseudopotential needs to be updated at each iteration (the effective potential Vef f is built with the electronic charge density) and this

makes it participate to the screening process, further increasing its transferability. The prize to be paid to obtain the advantages introduced by US PPs (beside updating the DI

ij coefficients each time) consists in the fact that we need a very large cut-off energy

to describe the augmentation contribution to the charge density. However this term is important just in the calculation of n(r) and does not enter the diagonalization problem which has the dimension fixed by the (smaller) wave function energy cut-off.

### 1.4.1

### The non linear core correction

The PW PPs method is based on the assumption that the electronic charge density can be separated into a valence term nv(r) and a frozen core contribution nc(r). In its

original form H and xc potentials in the solid are calculated using nv(r) only. This is

not an approximation for the Hartree potential because it’s linear in the charge density and the contribution coming from the core term can be easily separated from the other (and included in the local part of the pseudo potential). The problem exists instead for the xc potential which is not linear in the density. Thus separating the xc energy density as

xc(nv(r) + nc(r)) ∼ xc(nv(r)) + xc(nc(r)) (1.54)

introduces a systematic error which is more serious when the two contributions to the charge density considerably overlap with each other. It follows that the systems having valence electrons strongly penetrating in the core regions (they usually are very localized external states like d bands for transition metals or f states in rare earths compounds)

with strong overlap with the valence ones in the valence manifold, but this would become very expensive from a computational point of view, also requiring a larger space for the wavefunctions to be stored. The non linear core correction (NLCC) approximately overcomes this difficulty including the core contribution in the charge density when computing the xc energy and potential. The xc energy thus results:

Exc[nv+ nc] =

Z

(nv(r) + nc(r))xc(nv(r) + nc(r))dr (1.55)

where the core contribution is still fixed in its frozen atomic configuration (it is not updated during iteration). The need of introducing the NLCC formalism is particularly evident when dealing with magnetic crystals: without including the core contribution (which is spin unpolarized), into the charge density, the magnetic polarization ξ, intro-duced in eq. 1.28,

ξ(r) = n↑− n↓

n↑_{+ n}↓ (1.56)

could be significantly overstimated thus spuriously enhancing the tendency of the system to acquire a finite magnetization.

### Some

_{d-open shell systems studied}

### with GGA

### 2.1

### introduction

The present chapter is devoted to the study of selected compounds using standard DFT
methods. All the chosen systems contain Iron whose electronic configuration (for the
isolated atom) is [Ar]3d6_{4s}2_{. Both the 3d and the 4s electrons of iron (which populate}

the most external shells) play an important role in the chemistry of this element. Being weakly bound to the ionic core (composed by the nucleus and the most internal electronic clouds) the 4s electrons are easily lost by the atoms in presence of other elements with (even slightly) higher electronegativity (as oxygen, for instance). A different behaviour is observed instead for the 3d electrons which, being more localized than the 4s ones, are more bound to the ionic cores. Despite this fact, they are deeply involved in the chemical bonds that ions form and, being usually the highest energy occupied states, they are frequently responsible for the conduction properties of iron compounds, as they represent the incomplete manifold crossed by the Fermi energy. However, despite the fact that the electrons which are responsible for the possible metallic behaviour of iron compounds are mainly accommodated on these states, the d levels strongly retain their atomic character which (usually) produces quite narrow bands, very localized charge densities and magnetic moments.

The localization of the d (open) shell electrons may cause electronic correlations on the atomic sites to play a very important role in the physical behaviour of iron (and, in general, of transition metal) compounds and create some troubles to conventional LDA or GGA approaches which are not designed to deal with rather localized strongly

The motivation of the present chapter is thus twofold: from one side we study the physical properties of some representative systems that are correctly addressed within GGA and whose good description we would like to be preserved (as much as possible) also when using our LDA+U scheme; on the other hand we can consider the aspects that are not well reproduced by the conventional xc functionals and possibly need a better treatment of the electronic correlations.

The chapter is divided in three sections each one devoted to a different material: (bulk) iron, FeO iron oxide and Fe2SiO4 fayalite.

The computational approach adopted to study these compounds is GGA used in its spin polarized version together with NLCC. For each of these systems, we present the band structure, the magnetic moment arrangement, and the structural properties (determined from the fit of our total energy calculations to the Murnaghan’s equation of state) and comparison is made with the experimental results (when available) to underline successes and defects of this preliminary study.

Bulk iron has been studied extensively using ab-initio calculations and we know that σ-GGA together with NLCC pseudopotentials are required to obtain the bcc ferromag-netic (FM) phase as the ground state (LDA without NLCC predicts a paramagferromag-netic fcc structure to be the most stable) [25]. Within this approximation it is quite well de-scribed by standard DFT which is able to correctly reproduce structural, magnetic, and also vibrational properties [26]. Thus the strong correlations existing for the d electrons around the Fermi level are not expected to be very important for this material and this is the aspect we want to investigate in this thesis.

Iron oxide, FeO, (as many other transition metal oxides) is a material which can be poorly described within GGA. Even if this theoretical approach can give reasonably good results for the magnetic moments and the equilibrium lattice spacing, it is less accurate in describing its behaviour under pressure (in particular the distortion along the [111] direction) and, more seriously, fails in reproducing the observed insulating ground state. In fact, as other compounds of this class (the transition metal oxides), FeO is an insulator of supposedly Mott kind where the band gap is actually due to the strong on site Coulomb repulsion which forbids the electrons to hop from one site to another. The approximated expression of the conventional GGA functionals is thus not sufficiently accurate to give a good description of the electronic properties of this compound, and this is probably the reason for the failure in describing its physical behaviour which will be presented in this chapter.

Fe2SiO4 fayalite is a mineral of geophysical interest in the study of the Earth’s upper

mantle. We present some calculations (using, in this case, both LDA and GGA) for this compound and we eventually obtain both magnetic and structural properties in quite good agreement with experiments (the best results were produced by GGA). However, despite the observed insulating behaviour, we obtain a metal with a narrow band of iron d-levels crossing the Fermi energy. The charge density of the states around this level was found to be extremely localized on iron sites thus revealing the strong atomic-like character of these electrons and the possible importance of on site correlations. Comparing GGA calculations to a simplified Hubbard model we will be able indeed to roughly estimate the average Hubbard U , and to obtain a value of 2.4 eV consistent with a Mott-Hubbard behaviour of this compound.

### 2.2

### Bulk iron

In this paragraph we report some results about the equilibrium structural, magnetic and electronic properties of bulk iron as obtained by DFT calculations.

In order to describe electron-ion interactions we use an ultrasoft pseudopotential generated according to a modified Rappe-Rabe-Kaxiras-Joannopoulos (RRKJ) scheme [27] which has been used previously in a structural and vibrational study of iron [26]. As the LSDA is known to give wrong results about the ground state structural properties of this material, we adopt the σ-GGA framework using the Perdew-Burke-Ernzherof (PBE) [13] expression for both the exchange and correlations functionals. An energy cut off of 35 Ry is chosen to describe the electronic pseudo wavefunctions while the augmented part of the charge density is expanded up to 420 Ry. The wave function energy cut-off is larger than the one used in other works for iron [26], but this will be required in LDA+U calculations and we adopt the same choice here in order to obtain consistent results in both schemes. To perform reciprocal space integrations we adopt the Monkhorst and Pack special point technique [14] and a mesh of 8×8×8 special points (corresponding to 29 inequivalent points within the Irreducible wedge of the Brillouin Zone) is found to sample the BZ quite accurately. The Methfessel and Paxton smearing technique [18] is used to smooth the Fermi distribution and a broadening of 0.005 Ry, which is smaller than required in ”ordinary” DFT calculations, gives good accuracy for our LDA+U calculations whose results will be presented in the last chapter and compared with the ones obtained in this section.

60.0 70.0 80.0 90.0 100.0 110.0 Volume -0.1 0.0 0.1 0.2 0.3 0.4 Energy (eV)

Figure 2.1: The fit to the Murnaghan equation of state for bcc FM Iron. The volume is
given in (a.u.)3 _{while the zero of the energy coincides with the minimum of the }

energy-volume fit.

Table 2.1: The calculated lattice constant (a0), bulk modulus (B0) and magnetic moment

(µ0) in comparison with LSDA (from ref. [26] and experimental results (from ref. [28].)

a0 (a.u.) B0 (Mbar) µ0 (µB)

σ-GGA 5.42 1.45 2.46

LSDA 5.22 2.33 2.10

Expt. 5.42 1.68 2.22

a body centered cubic structure. In order to study the structural properties of this FM bcc phase, we change the volume of the unit cell (while keeping its cubic shape fixed) and study the behaviour of the total energy of the system. The result is shown in fig. 2.1 where a fit of the calculated points to the Murnaghan equation of state is also introduced to estimate the equilibrium lattice spacing and the bulk modulus. In table 2.1 a comparison is made between the experimental and the theoretical results

### Energy [eV]

### -10

### -5

### 0

### 5

### 10

### 15

### H

### P

### Γ

### H

### N

### P

### N

### Γ

Figure 2.2: The band structure of bcc iron. Solid line for majority spin bands, dotted line for minority spin bands. The 0 of the energy is set at the Fermi level. The experimental results were taken from [55].

for these quantities and for the magnetic moment on each ion. The agreement with the experiments is fairly good for the cell parameter, while there are large discrepancies (but much smaller than those produced by LSDA [26]) for the bulk modulus and the magnetic moments. The electronic structure obtained at the equilibrium lattice parameter is

-10.0 -5.0 0.0 5.0 10.0 15.0 3.0 2.0 1.0 0.0 1.0 2.0 3.0 s states (x 5) d states Energy (eV) DOS (states/eV/cell)

Figure 2.3: The projected density of states of bcc iron. Red lines are for d states, black lines for s states. The top panel is for majority spin states, the down panel for minority spin states. The s density of states is multiplied by a factor of 5 in order to have an integral comparable with the one of the d density of states.

shown in fig. 2.2 where a finite splitting among the two spin populations (which is the origin of the ferromagnetic character of the material) is evident and larger in the region around the Fermi level. In the same plot some experimental results obtained by photoemission techniques by Turner et al. [55] are also shown. The comparison with our calculated band structure seems to be quite good especially in the Γ-N-P region, while a somewhat looser correspondance is obtained around the H point and in the Γ-P-H zone. In this plot a clear distinction can be made among two groups of levels as also evident from the projected density of states in fig. 2.3: the first group, extended in the region around the Fermi energy (approximately from 5 eV below the Fermi energy to 3eV above it), is mainly composed by the 3d levels of iron; the second group, with a much larger dispersion, consists of the 4s states which extend between 8 and 4 eV below

the Fermi level, and above the region occupied by the d states. The magnetization of the ions (generated by the relative shift among the two spin populations) is due, to a large extend, to the d states. Thus, the same electrons which are responsible for the metallic behaviour, also give rise to the magnetic properties of this material (itinerant ferromagnetism). However a very small contribution also comes from the s states because, as it can be observed in figure 2.3, they have slightly different density of states in the two spin channel which produces unbalance among their populations (the integrals of the two density of states are 0.39 and 0.45 electrons/cell for the majority and the minority spin s states respectively). As it can be observed from fig. 2.3, in the region around the Fermi level states of both kind coexist, but the s density of states is strongly depleted (for both the spin channels) in the region where the d levels are located, and is quite small in proximity of the Fermi level. The mixing among the two is thus expected not to be very important so that the metallic character of the material mainly arises from the strongly atomic-like d states.

As evident from the study about electronic, magnetic and structural properties, the GGA approach gives a very good description of bulk iron; some questions, however, still remains about its physical behaviour as, for instance, the mechanism which leads to atomic like magnetic moments. The magnetism produced by itinerant electrons, in fact, is still an open problem and the importance of the electronic correlations in this context is one of the points under debate [29].

### 2.3

### Iron oxide

Iron oxide (FeO) is a much more problematic material than Fe to be studied with state-of-the-art numerical techniques. As it happens in most transition metal oxides, LDA completely fails in reproducing the observed insulating behaviour (expected to be produced by a Mott-like mechanism); nevertheless it can describe the structural and magnetic properties of this compound in reasonable agreement with experimental results, at normal pressure and temperature conditions.

In this paragraph some results of a σ-GGA study of FeO will be presented and particular care will be devoted to its structural and electronic properties, to be compared with the LDA+U results presented in a later chapter of the thesis.

The calculations are performed describing iron with the same US GGA (PBE) NLCC pseudopotential already used for the bulk material, while for oxygen an US PBE (non NLCC) potential has been chosen. The same smearing amplitude (0.005 Ry) as for bulk

Figure 2.4: The unit cell of FeO. Red balls are Fe, blue are O, while the arrows represent the spin polarization of the magnetic ions

iron is also used to smooth the Fermi distribution (we know that GGA describes this compound as a metal) and a 4×4×4 mesh k-points (corresponding to 13 independent vectors within the IBZ) is found to be enough for reciprocal space summations. An energy cut-off of 40 Ry is chosen to describe the electronic wave functions, while the augmented contribution to the charge density requires a 400 Ry cut-off. These are again larger values than strictly required in ”normal” GGA (or LDA) calculations, but we choose them in order to compare directly these results with those obtained in LDA+U approach in which they are necessary.

The unit cell of FeO (in the undistorted phase) has a cubic rock salt (B1) struc-ture with rhombohedral symmetry originating from the magnetization of the iron. The ground state spin configuration, shown in fig. 2.4, is ferromagnetic for ions belonging to

220.0 260.0 300.0 340.0 380.0 Volume -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 Energy [eV]

Figure 2.5: The fit to the Murnaghan equation of states for iron oxide. The volume is
given in (a.u.)3 _{while the zero of the energy coincides with the minimum of the }

energy-volume fit.

the same [111] planes, while nearest neighbor magnetic planes are in an antiferromag-netic configuration with each other because of a superexchange interaction mediated by the oxygen ions lying in between [30]. At ambient pressure a rhombohedral stretching of the crystal structure along the [111] body diagonal is also observed upon lowering the temperature below the N´eel value (≈ 198 K). The distortion is found to increase under pressure loading and the N´eel temperature is also observed to increase; at higher pressure the system transform to other structural phases whose nature has been recently studied [31, 32] and which will not be addressed here. We begin studying the undistorted structure in the ground state rhombohedral AF spin configuration. The results of our calculations can be seen in fig. 2.5 where the curve resulting from a Murnaghan fit to the calculated points is also drawn and used to extract some structural parameters of this material. In the table 2.2 a comparison is made with the experimental results about the lattice parameter, the bulk modulus and the magnetic moment of each iron. Despite some scattering in the experimental results, the agreement is reasonable especially for

(µ0) in comparison with experimental results (taken from ref. [31].)

a0 (a.u.) B0 (Mbar) µ0 (µB)

σ-GGA 4.30 1.73 3.61

Expt. 4.33 1.42-1.80 4.20

the lattice parameter (we report the side of the conventional cubic cell of fig. 2.4 which is not a fundamental direct lattice vector) and the bulk modulus. A larger discrepancy is obtained for the magnetic moment of each iron which is anyway in better agreement with experimental result than in other theoretical studies [31].

The electronic band structure of iron oxide has been calculated at the equilibrium lattice parameter (of the undistorted cubic structure) for the AF spin configuration depicted in fig. 2.4. The result is plotted in fig. 2.6 where the zero of the energy scale is set to the Fermi energy. As it can be noticed from the plot, there is a complete degeneracy among the spin up (solid lines) and the spin down (dotted lines) electronic levels due to the antiferromagnetic ground state spin configuration. The majority spin d states of each iron are located between 4 and 1 eV below the Fermi energy, while the (partially filled) minority bands are extended around the Fermi level (between -1 to 2 eV) and cross it in several points thus producing the metallic behaviour. This is at variance with experimental results which show an insulating ground state for this compound at low pressure and temperature, and represents the most evident failure of LDA (or GGA) in describing this class of compounds. However, the itinerant character of the d electrons of iron is not in contradiction with the non zero magnetization which actually results from the finite (exchange) splitting between majority and minority spin states. Thus, while failing in reproducing the conduction properties, LDA and GGA can give appreciable results about the magnetization on each ion. Four groups of states in the electronic band structure can be distinguished: the oxygen s and p states lying at about 20 eV and between 9 and 4 eV below the Fermi energy respectively, the iron d levels from -4 to 2 eV around the Fermi energy, and the iron s states which are completely empty in the region above the Fermi level. In a perfectly cubic environment the d states of the magnetic ions could be further divided into two subgroups: the low lying t2g levels (xy, yz and xz) and the higher energy eg states (x2− y2 and 3z2− r2).

### Energy [eV]

### -20

### -15

### -10

### -5

### 0

### 5

### Γ

### L

### K

### T

### Γ

### X

Figure 2.6: The band structure of iron oxide corresponding to the spin configuration of fig. 2.4. Solid lines, for majority spin bands, are completely degenerate with the dotted line for minority spin bands. The zero of the energy is is set to the Fermi level.

t2g degeneracy of the cubic structure and produces one state of A1g symmetry, which

corresponds to the linear combination _{√}1

3(xy + yz + xz) of 3Z

2_{−r}2 _{symmetry where Z is}

taken along the [111] rhombohedral axis, and two other states of Eg symmetry lying on

the FM [111] planes corresponding to E1

-20.0 -15.0 -10.0 -5.0 0.0 5.0 Energy (eV) 0.0 1.0 2.0 3.0 4.0 5.0 6.0 7.0 DOS (states/eV/cell) Fe d up states Fe d down states O s states O p states

Figure 2.7: The projected density of states of AF undistorted iron oxide. The zero of the energy is set to the Fermi level.

insulating gap could not be realized without rhombohedral symmetry [31] [33] because in this case the degenerate t2g states would all sit at the Fermi level thus producing a

1/3 filled band. In the rhombohedral symmetry, in order the gap opening to take place, the A1g state should correspond to a lower energy with respect to the other two states

originating from the t2g triplet (the six d electrons of iron would completely fill in this

case the five majority spin states and the lowest energy minority-spin state thus leaving the other states above the Fermi energy). This is not realized within the GGA which thus also fails in ordering the d orbitals of the magnetic ions. Furthermore, even if this order were correct, the gap in the band structure would have been too small [31] (as it happens for MnO and NiO) because it is not just produced by the ligand field acting on the iron, but rather it is expected to be due to electronic correlations which are not properly described within ”ordinary” mean-field-like LDA or GGA approaches.

A related aspect which is, however, somehow well described by GGA calculations is the spectroscopical nature of the (unrealized) gap opening at the Fermi level:

pho-225.0 235.0 245.0 255.0 265.0 275.0 285.0 295.0 Volume -0.1 0.0 0.1 0.2 0.3 0.4 0.5 0.6 Energy [eV] 63.34 60.00 56.72 53.49 50.29

Figure 2.8: The Murnaghan fits for different distorted structures. smaller angles
corre-spond to larger rhombohedral distortions. The volume is given in (a. u.)3_{.}

toemission and optical experiments on iron oxide both reveal that the valence band of this compound is of mixed O 2p-Fe 3d character [33] so that transitions between the valence and the conduction band should also involve electrons hopping from oxygen to iron (charge transfer insulator). A strong mixing between the oxygen p states and the iron d levels should therefore be observed on the top of the valence band. Despite the gap is not obtained within GGA, the mixing among these states is somehow realized in our calculation as evident from fig. 2.7 where the projected density of states describ-ing different atomic contributions has been plotted. Neglectdescrib-ing the states at the Fermi energy, mainly originating from the minority-spin d states, we can see, in fact, that a considerable overlap of oxygen p states and majority-spin d states exists in the region near to 2 eV below the Fermi level. However, the spectral weight of this overlap region is mainly due to iron d levels while a stronger interaction among oxygen p and iron d states can be observed only between 5 and 9 eV below the Fermi level where oxygen states give the ominant contribution. In other words, even if some finite overlap exists, the two atomic contributions are centered in different regions of the energy spectrum.

### α

rFigure 2.9: The rhombohedral angle is the one among any two of the face diagonal
vectors. In the undistorted structure its value is 60◦_{.}

Despite GGA is quite successful in reproducing the lattice spacing and the bulk mod-ulus of FeO in the cubic (undistorted) structure, the failure in describing its electronic properties is possibly the reason of quantitatively wrong results for the rhombohedrally distorted phase. In fact the cubic structure of FeO is found to be unstable with respect a rhombohedral stretching along the [111] cubic diagonal and the reason of this is a strong interplay among electronic/conduction properties, orbital ordering, and crystal symmetry, producing very efficient magnetocrystalline interactions [31]. In fact, the dis-tortion is observed at ambient conditions when temperature is decreased below the N´eel threshold (which is of about 198 K) and found to even increase under pressure loading. The GGA approach to the study of FeO correctly predicts the distorted structure to be the ground state at normal conditions (calculations are always performed at zero tem-perature) and also reproduces the enhancement of the rhombohedral stretching under pressure loading. In fig. 2.8 the fitting curves corresponding to different rhombohedral distortions are plotted (the distortion parameter is the rhombohedral angle αr among

any two face diagonal vectors shown in fig. 2.9) and it can be seen that increasing pres-sure favours larger and larger distortions. In order to study the increase of distortion from a quantitative point of view we calculated the pressure corresponding to each point of the Murnaghan curves and explored a pressure range from 0 to 200 kbars. At each chosen pressure (we divided this interval in 20 parts) we calculated the enthalpy of the

0.0 50.0 100.0 150.0 200.0 Pressure (kbar) 51.0 52.0 53.0 54.0 55.0 56.0 57.0 58.0 59.0 60.0

Rhombohedral angle (degrees)

Exp GGA

Figure 2.10: The rhombohedral angle as a function of pressure.

system (E + P V ) and fitted its dependence on cos αr with a quadratic curve finally

obtaining the rhombohedral angle corresponding to the minimum of the enthalpy. The
result is shown in fig. 2.10 where a clear tendency toward the enhancement of the
rhom-bohedral distortion can be observed as predicted by [31] and references quoted therein.
In the same picture two experimental points are also presented. The ambient pressure
experimental result was extracted from ref. [34], whereas the 200 kbar one was obtained
from ref. [35]. Both of them were obtained for non stoichiometric compounds so that
we extrapolated the experimental results up to the composition with the same amount
of iron and oxygen using the linear dependence of the rhombohedral angle with iron
concentration obtained in ref. [34] from measurements at 90 K and ambient pressure.
The use of the same linear dependence on ion concentration may not be very accurate
for the point at 200 kbars. In any case the amount of stretching (the deviation of the
rhombohedral angle from its cubic structure value of 60◦_{) predicted within GGA is far}

too large if compared with experimental points even if we consider the results obtained for the non stoichiometric compound which is used in experiments. In ref. [36] the same agreement with experimental results led the authors to conclude that the behaviour of